Carbon Fiber Composite Body Structures Viper Reports
Embed Size (px)
Transcript of Carbon Fiber Composite Body Structures Viper Reports
CARBON FIBER COMPOSITE BODY STRUCTURES
FOR THE 2003 DODGE VIPER
Mark Bruderick, Douglas Denton and Michael Shinedling, DaimlerChrysler Corporation and Michael Kiesel, Quantum Composites Inc.
The first automotive application of carbon fiber sheet molded composite (CFSMC) is made in nine components of the 2003 Dodge Viper Convertible to provide structural performance and to achieve significant weight savings. Right and left fender support systems employ a total of six carbon fiber composite moldings. In addition, carbon fibers are used to provide selective stiffening to the windshield frame and door inner structures, which consist primarily of conventional glass fiber SMC (GFSMC). The design and analysis, CFSMC materials and process, and performance of these innovative composite structures are discussed.
Introduction The primary objective of DaimlerChrysler Performance Vehicle Operations for the development of the all new 2003 Dodge Viper Convertible was maximizing vehicle performance while maintaining low vehicle mass. An important consideration in the vehicle development was the judicious application of new technologies that potentially can be extended to higher volume car and truck lines. Consequently, the new Viper makes innovative use of compression molded carbon fiber SMC in several break-through body structure applications. A total of eight kilograms of carbon fiber composite is used in nine body components. Glass fiber reinforced composites have been used for decades in the automotive industry to provide light-weight structures with reduced capital investment. Composites provide additional advantages such as parts consolidation, design flexibility, and corrosion resistance. Carbon fiber composites offer the possibility of even greater weight savings than glass fiber composites, but the cost of the material is significantly higher. As a result, they have typically been applied in very limited applications using processes capable of very small volumes (under 1000/year). The 2003 Viper is the first use of a materials system and process capable of higher volume production (100,000+/year). While carbon fiber SMCs have been commercially available for 16 years, the application of these materials in the automotive industry have been slow to develop due to the high cost of carbon fibers, and the lack of understanding of carbon fiber composites. Recent developments at carbon fiber supplier companies have reduced costs and hold promise for further price reductions (1). In addition, programs under the sponsorship of the U.S. Department of Energy are exploring methods to fundamentally change the production of carbon fibers to reduce their cost (2). Work within the Automotive Composites Consortium and studies at the Oak Ridge National Laboratory are providing a better understanding of the performance and durability characteristics of commercial grade composites containing carbon fibers (3,4). All of these efforts are increasing the feasibility of using carbon fiber composites in the automotive industry. Three Viper structural systems that employ the high modulus of carbon fiber SMC to achieve exceptional stiffness in lightweight structures are presented in this paper. Thin-wall sections in the six-piece fender support system provide numerous functions at a minimum weight. The hybridization of random CFSMC with low-density glass SMC improves the stiffness of structural inner panels to minimize door sag. And the blending of SMC containing continuous oriented carbon fibers with high glass content structural SMC in the windshield frame provides stiffness to resist deflections.
Figure 1. Carbon and Glass Fiber Composites on the 2003 Viper
= Glass Fiber Composites
= Carbon Fiber Composites
Door Inner Panel R&L (Carbon-Glass Hybrid)
Fender Supports R&L
Carbon Fiber-Vinyl Ester SMC
Carbon fiber SMC is compounded and molded in a manner similar to conventSMC. The Viper parts use two CFSMC materials produced by Quantum Compositoughened vinyl ester resin with 25 mm random chopped 12K PAN (polyacrylonitAMC-8595 contains a continuous, unidirectional cross-stitched mat with the same toughened vinyl ester matrix as AMC-8590. All of the Viper components containing AMC-8590 and AMC-8595 are coAutomotive Systems in Shelbyville, IN. CFSMC cures at conventional tempera(1-3 minutes). AMC-8590 requires 70%-90% of the mold be covered with the AMC-8595 does not flow in the fiber direction. Consistent charge preparation structural performance of the molded part. The primary advantages of carbon fibers in SMC are higher modulus and lower speThe modulus of commercial-grade carbon fibers is approximately 230 GPa, which E-glass fibers. In addition, the 1.8 specific gravity of carbon fibers is about 70% ofThese fiber properties translate into thinner and lighter composite structures. With surround, nominal part thicknesses ranged from 2.0 to 2.5 mm. Properties of the Qpresented in Tables 1 and 2.
Windshield Frame Outer and Inner Panel(Carbon-Glass Hybrid)
Headlamp Supports R&L
Sill to Fender Brackets R&L
ional structural-grade glass fiber tes, Bay City, MI. AMC™ 8590 is a rile) based carbon fiber tows. 12K carbon fibers and the same
mpression molded by Meridian tures (145-155°C) and cure times
charge to minimize flow lines. and placement are critical to the
cific gravity relative to glass fibers. is more than three times higher than the specific gravity of glass fibers. the exception of the windshield uantum Composites CFSMCs are
Table 1. Properties of Quantum Composites AMC-8590 (Random chopped carbon fibers)
Property Method Net Shape
Specimens Cut From Panel,
Specimens Cut From Panel,
Fiber Content (% by weight) Solvent Wash 55% Specific Gravity ISO 1183 1.48 Tensile Strength (MPa) ISO 527 212 134 ASTM D 638 287 Tensile Modulus (GPa) ISO 527 42.2 32.5 ASTM D 638 55.0 CTLE (mm/mm/°C) ASTM D 696 6.17 x 10-6 5.54 x 10-6
Heat Deflection Temp. @ 1.80 MPa Stress (°C) ISO 75 >260
a – Molding induces fiber orientation in the specimen direction and cuts fewer fibers. Table 2. Properties of Quantum Composites AMC-8595 (Continuous oriented carbon fibers)
Property Method Specimens Cut From Panel, Machine/ Fiber Direction
Fiber Content (% by weight) Solvent Wash 55 Specific Gravity ISO 1183 1.49 Tensile Strength (MPa) ASTM D 3039 1200 Tensile Modulus (GPa) ASTM D 3039 120 CTLE (mm/mm/°C) ASTM D 696 9.47 x 10-7
Heat Deflection Temp. @ 1.80 MPa Stress (°C) ISO 75 >260 AMC™ is a Trademark of Quantum Composites, Inc. Figure 2. Materials Comparison - Typical Property Averages
Tensile Strength Tensile Modulus (Stiffness)Typical GFSMC 10.25 11.67R55 CFSMC 33.34 48C55 CFSMC 139 104
Tensile Strength Tensile Modulus (Stiffness)
Windshield Frame Evolution of the Composite Windshield Frame - From Viper to Prowler to Viper
The new 2003 Viper uses a composite windshield frame as was introduced on the original Viper and the Plymouth Prowler. The design incorporated by the new Viper represents a further step forward in the evolution of the composite windshield frame. Composites were chosen for this application because of the lower tooling cost and part consolidation benefits.
The 1992 Viper used RTM composite technology on the windshield surround. The design included random
glass pre-forms wrapped around a foam inner core with steel reinforcements and molded in a single cavity. This process required extensive hand finishing particularly around the eight parting line edges of the part.
The 1997 Prowler used a new patented application for the windshield frame. The Prowler design consisted of a
two-piece glass SMC surround bonded together with structural adhesive. The bond seam required hand finishing on four edges of the part. SMC offered greater design flexibility and part consistency than RTM. The Prowler surround used unidirectional glass SMC in the A-Pillars to maximize stiffness and was able to achieve a 9% improvement in bench stiffness compared to the outgoing Viper. The 2003 Viper adopts a Prowler-type windshield frame because of its design advantages. The new car also further refines the two-piece SMC design by limiting the hand finishing to only one edge (rear header) of the part and increasing part stiffness. Figure 3. Windshield Frame Components and Materials
Unidirectional Carbon Fiber orientation in each A-Pillar
Glass Fiber SMC with 0.46 kg Carbon Fiber SMC
(0.23 kg per A-Pillar)
Glass Fiber SMC with 0.46 kg Carbon Fiber SMC
(0.23 kg per A-Pillar)
Windshield Frame CFSMC content: 0.92 kg
Styling Challenges and Federal Requirements The styling on the 2003 Viper angles the windshield further back and increases the A-Pillar length to 610mm; nearly 25% longer than the Prowler and original Viper (495mm and 490mm respectively). The new federally mandated head impact requirement drove the addition of energy absorbing A-Pillar trim covers on the interior. This decreased the cross-section area for added stiffness. In order to achieve the performance objectives the engineering team turned to carbon fiber SMC. Each windshield frame contains 0.92 kg of unidirectional carbon fiber SMC. The unidirectional fibers are oriented along the length of the A-Pillars in both the inner and outer panels. The fibers are layered in the section to maximize stiffness and minimize appearance effects. The total weight of the surround is 8.9 kg. Figure 4. Windshield Frame A-Pillar Cross Section Performance Results The 2003 Viper windshield surround has 45% less bench test deflection than the original model. Factoring in the longer A-Pillar, this is a 122% increase in normalized stiffness.
Class-A Surface (low gloss paint)
Outer Panel Glass Fiber
Inner Panel Glass Fiber SMC
Unidirectional Carbon Fiber
A-Pillar Trim Thermoplastic
Glass-Carbon Hybrid Door Inner Panel
Challenges of a Viper Door A styling trademark on Viper is the large “gill” opening on the body side just behind the front wheels. This gill opening creates an unconventional door cut-line that limits the hinge pillar surface to nearly half the height of the door. This in turn increases the moment load on the hinges and the front section of the door inner. The original Viper and the 2003 model both use only a single hinge per door. The original Viper doors were constructed of RTM outer and inner. The original doors used large steel panels on the hinge pillar and latch pillar for strength and stiffness. The intention for the new car was to decrease the cost,
complexity and weight of the doors by using Class A SMC, low density SMC and smaller steel reinforcements. However, further enhancements were needed to meet all of the performance objectives. Performance Requirements During the development of the door the critical performance criteria were door sag deflection and permanent set. Door sag is the maximum deflection measured on a door in the open position with a specified load applied. Permanent set is the deflection measured after the door sag load is removed. A new technique of blending random carbon fiber SMC and glass fiber SMC was developed to improve the performance of the door in these two areas without increasing the size of the steel reinforcements. Figure 5: Door Component Materials
Hinge Pillar Reinforcement (Steel) Bonded to Inner Panel
Glass SMC Outer Panel
LD Glass SMC
Blended Substrate Area
Carbon Fiber SMC
0.45 kg per door
Door CFSMC content per vehicle: 0.9 kg Hybrid Blending of CFSMC and GFSMC The door inner design called for blending carbon and glass materials to maximize on stiffness in the high strain energy areas at a minimum cost. The front portion of the door (20%) would be made up entirely of carbon fiber SMC and the rear portion of the door (80%) would be made up of low density SMC containing glass fibers. This hybrid blending in the door presented a more difficult challenge than the windshield surround. The windshield surround glass fiber materials complete enveloped the reinforcing carbon fibers. In the case of the door panel, a transition from the CFSMC to the GFSMC is required in the plane of the part. A study of different blending techniques was performed to determine the optimum joint for molding these two materials together. The strength, dimensional accuracy and processability of the joint were the main considerations. This study focused primarily on two methods of blending equal volumes of carbon fiber SMC with low-density glass fiber SMC to form a molded “joint.” In the first, the GFSMC and the CFSMC are overlapped in the mold charge by either 25 mm or by 50 mm. In the second, GFSMC is inserted by either 25 mm or 50 mm into the two ply stack of the CFSMC. Plaques containing only carbon fiber SMC or glass fiber SMC were molded as controls. The charge patterns, covering 55% to 70% of the 305 mm x 305 mm mold, were molded into uniform 2.5 mm thick panels. Flow of the SMCs generally caused the transition zones to double in length. In cross-section the molded overlap joint appeared to approximate a single scarf joint, where as the insert joint approximated a double scarf joint. Straight edged tensile bars measuring 25 mm x 305 mm were cut with a diamond tipped blade and tested in general accordance to SAE J2253 / ASTM D5083.
Figure 6: Material Charge Pattern Configurations for the CFSMC to GFSMC Transition CFSMC
GFSMC Overlap Joint Insert Joint Figure 6. Transition of carbon fiber composite to glass fiber composite in molded parts. . Overlap Joint Insert Joint
A summary of tensile strength data is presented in Figure 7. Six specimens were tested at each condition. It is
evident that the strength and the variation are much greater for the carbon fiber SMC than for the glass fiber SMC. The coefficients of variation are 23.2% and 6.1%, respectively. The strengths of the four different configurations are all statistically equivalent to the strength of the glass fiber SMC. Thus, it appears that stress concentration caused by the interface between the two dissimilar materials is not reducing the tensile strength below that of the glass fiber SMC. However, it was noted that most fractures occurred at the interface between the two different SMCs. While strength did not differentiate the two types of joints, it became evident from visual examination of the panels that out-of-plane distortions were different. Individual panels were fixed along one edge and the deviation of the opposite two corners was measured. This revealed that the asymmetric joint, the overlap, resulted in nearly a four-fold greater deviation from plaque planarity than the symmetric “insert” joint. Results of this study were used in the design of the charge pattern for the door inner panels. Figure 7: CFSMC / GFSMC Transition Study Results (brackets indicate +/- one standard deviation)
69.3 68.1 69.3 67.1 70.7
CFSM CContro l
O verlap25m m
O verlap50m m
Insert 25m m Insert 50m m G FSM CContro l
Performance Results The final construction of the door yielded a 206% improvement in door sag stiffness and a 350% improvement in resistance to permanent sag deflection. Reducing the size of the steel reinforcements gave a weight savings of approximately 3 kg.
Fender Support System Design Concept The front-end of the original Viper was made up of a one-piece clamshell hood. With a multiple piece inner panel, excessive hand finishing, and its massive size, the hood was a very difficult part to manufacture. The styling of the 2003 Viper would offer the advantage of a traditional hood and fenders, keeping however the same space-frame chassis architecture. Many different options were considered to attach the new hood and fenders to the Viper space-frame including local stamped brackets, tubular metal reinforcements and fender inner panels. The engineering team decided to investigate new materials and a new concept for supporting the front end of the vehicle. Carbon fiber SMC was ultimately chosen as the material for the new front-end fender support system. This process and material gave the design team great flexibility in consolidating brackets and increasing the function of the system. The initial design intent was to create one left and one right molded panels that would support the fender, the headlamps, and provide the dimensional reference for the entire front end of the Viper body. The design evolved into three molded panels per side: a fender support; a headlamp support; and a sill to fender bracket. Each of these panels would be molded out of carbon fiber SMC. The panel break up was driven by two main factors: 1. Minimize complexity of the molding tools; 2. Provide serviceability of the headlamp supports and the sill to fender brackets (areas of the system most likely to be damaged in a minor collision). Figure 8. Fender Support System Components
Headlamp Extension 0.80 kg each
Fender Support Panel 1.93 kg each
Total carbon fiber content = The fender support system is constructed by first bonding the headlamp supadhesive. This sub-assembly is next water jet cut and final assembled with f
Sill-To-Fender Bracket 0.34 kg each
.14 kg per vehicle
rt to the fender support with structural steners. The fender support assembly
is located to the vehicle by four net-form-and-pierce locations on the frame and two small locating fixtures. The fender supports are bonded to the frame by structural urethane adhesive and mechanically fastened with four screws and two nuts. Finally, each sill-to-fender bracket is fastened to the fender support assembly with three rivets. Evolution The fender support system increased in functionality as it evolved. The design flexibility of SMC allowed additional attachments at a minimum cost without adding panels and brackets. The fender supports use molded embossments, U-Nuts, Rivet-Nuts, Rivet-Studs and snap-in features to provide attachments for the following components: Fenders, Side Sills, Hood, Fascia, Headlamps and Cowl Screens. Attachments for several under-hood components were added to the fender supports. On conventional body-in-white, most of these attachments would have required separate brackets in order to gain the same functionality. Figure 9. Fender Support Under-Hood Component Attachments
Various Wiring Harnesses
Fog Lamp Access Covers Engine Controller
Oil, Radiator Coolant, and AC Lines
Hood Side Bumpers
Hood Prop Stud
Hood Slam Pads
Fuel Purge Solenoid
Power Center and Fuse Panel
Clutch Fluid Reservoir
Washer Fluid Bottle and Hose Routing
Brake Cooling Ducts
Cooling Pressure Bottle
Performance The bonding of the fender support assemblies creates an upper torsional load transfer path to the frame. The fender supports also provide structural stability to the magnesium front-of-dash near the center of the car. FEA studies show that the fender supports increase the front-of-dash and A-Pillar stiffness by 22%, and increase the first bending mode by 3.1 Hz. The fender support system, which has an average section thickness of 2 mm, reduces the weight of the vehicle by approximately 18 kg. The system, which is made up of 6.14 kg of carbon fiber SMC, dramatically reduces the number of brackets and metal reinforcements on the front end. An estimated 15-20 metal parts would have been required to achieve the same functionality of the six molded carbon fiber panels in the fender support system.
The 2003 Viper makes first automotive application of carbon fiber SMC to a vehicle body structure. Both thin section structures of all-carbon fiber SMC and the tailored hybridization of carbon fiber SMC to reinforce glass fiber SMC moldings are demonstrated. Mass reductions and stiffness improvements are achieved in the fender support system, windshield surround structure and door inner panels. The commercial manufacture of these parts represents a milestone for automotive composite technology as the industry begins to explore higher volume applications for carbon fiber reinforcements. The introduction of carbon fiber in a familiar material form and process, SMC, provides a relatively easy transition from glass fibers to this high performance fiber.
Acknowledgements The authors express appreciation to other members of the Performance Vehicle Operations team that have been instrumental in the development of the carbon fiber SMC applications on the 2003 Viper including Saad Abouzahr, Sriram Chandramouli, Brian Fabio, Tim O’Hara, Dan Pearlman, Steve Rowden, Gary Slota and Paul Thomas. The efforts of the Quantum Composites and the manufacturing team at Meridian Automotive Systems to make this work successful are acknowledged.
References (1) A. Dry, “The Development of the Carbon Fiber Industry,” 42nd International SAMPE Symposium & Exhibition,
May 5 -8, 1997. (2) C. David Warren, “Carbon Fiber in Future Vehicles,” SAMPE Journal, Vol. 37, No. 2, March/April 2001. (3) R. G. Boeman, N. L. Johnson, "Development of a Cost Competitive, Composite Intensive, Body-in-White,"
Proceedings of 2002 Future Car Congress, Arlington, Virginia, June 3-5, 2002 (4) J. M. Corum, et al., "Durability-Based Design Properties of Reference Cross-ply Carbon-Fiber Composite,"
ORNL/TM-2000/322, Oak Ridge National Laboratory, April 2001